HAL Id: hal-02021279
Submitted on 15 Feb 2019
HAL is a multi-disciplinary open access
archive for the deposit and dissemination of
sci-entific research documents, whether they are
pub-lished or not. The documents may come from
teaching and research institutions in France or
abroad, or from public or private research centers.
L’archive ouverte pluridisciplinaire HAL, est
destinée au dépôt et à la diffusion de documents
scientifiques de niveau recherche, publiés ou non,
émanant des établissements d’enseignement et de
recherche français ou étrangers, des laboratoires
publics ou privés.
electrochemically made disordered Na3V2(PO4)2F3
Guochun Yan, Sathiya Mariyappan, Gwenaëlle Rousse, Quentin Jacquet,
Michael Deschamps, Rénald David, Boris Mirvaux, John Freeland, Jean-marie
To cite this version:
Guochun Yan, Sathiya Mariyappan, Gwenaëlle Rousse, Quentin Jacquet, Michael Deschamps,
Higher energy and safer sodium ion batteries via an electrochemically made disordered
Na3V2(PO4)2F3 material. Nature Communications, Nature Publishing Group, 2019, 10, pp.585.
Higher energy and safer sodium ion batteries via an
electrochemically made disordered Na
, Sathiya Mariyappan1,2
, Gwenaelle Rousse1,2,3
, Quentin Jacquet1
, Michael Deschamps2,4
, Boris Mirvaux1,2
, John William Freeland6
& Jean-Marie Tarascon1,2,3
The growing need to store an increasing amount of renewable energy in a sustainable way has rekindled interest for sodium-ion battery technology, owing to the natural abundance of sodium. Presently, sodium-ion batteries based on Na3V2(PO4)2F3/C are the subject of intense research focused on improving the energy density by harnessing the third sodium, which has so far been reported to be electrochemically inaccessible. Here, we are able to trigger the activity of the third sodium electrochemically via the formation of a disordered NaxV2(PO4)2F3 phase of tetragonal symmetry (I4/mmm space group). This phase can reversibly uptake 3 sodium ions per formula unit over the 1 to 4.8 V voltage range, with the last one being re-inserted at 1.6 V vs Na+/Na0. We track the sodium-driven structural/ charge compensation mechanism associated to the new phase and ﬁnd that it remains disordered on cycling while its average vanadium oxidation state varies from 3 to 4.5. Full sodium-ion cells based on this phase as positive electrode and carbon as negative electrode show a 10–20% increase in the overall energy density.
1Chimie du Solide-Energie, UMR 8260, Collège de France, 75231 Paris Cedex 05, France.2Réseau sur le Stockage Electrochimique de l’Energie (RS2E), Cedex FR CNRS 3459, Amiens 80039, France.3Sorbonne Université - 4 Place Jussieu, 75005 Paris, France.4CNRS, CEMHTI UPR3079, Univ. Orléans, Orléans 45100, France.5LRCS, Université de Picardie Jules Verne, 80039 Amiens, France.6Advanced Photon Source, Argonne National Laboratory, Argonne 60439 IL, USA.7Present address: School of Metallurgy and Environment, Central South University, Changsha 410083, China. Correspondence and
requests for materials should be addressed to J.-M.T. (email:email@example.com)
The development of new types of high-performance energy storage and conversion technologies is urgently needed to meet the growing demands for portable electronic equip-ment, electric vehicles, and large-scale smart grids1,2. Batteries, as
one of the most versatile energy storage technologies, play a central role in the transition from fossil-based fuels to renewable energy. While the Li-ion technology is a key enabler in the transport sector, it falls short in the stationary storage sector because of high cost linked to the limited abundance of lithium. Sodium-ion battery technology has recently aroused great inter-est, among all the scientiﬁc community, as a valid and more environmentally friendly alternative to Li-ion, owing to the abundance of sodium all over the planet3,4. Present sodium ion
systems rely on carbon as the negative electrode and of either Na-based layered oxides or polyanionic compounds as the positive electrode5–9. Through comparative studies, it has been
demon-strated that the Na3V2(PO4)2F3/C system presently offers both cycling stability and power rate advantages over systems using the Na-based layered oxide NaxMO2(where x≤ 1 and M = transition metal ion(s))9–12.
Thus, this paper further focusses on the polyanionic Na3V2 (PO4)2F3 positive electrode material, now on termed as NVPF, from which one can reversibly remove two sodium ions per formula unit via two-step redox plateaus of equal amplitudes centered at ~3.7 and ~4.2 V vs. Na+/Na0. Besides, NVPF elec-trodes offer a sustained reversible capacity of 128 mAh g−1 together with a speciﬁc energy of 500 Wh kg−1, while showing excellent capacity retention and rate capability9,13,14. However, to
make sodium ion cells based on NVPF technologically relevant, there is a need to increase their speciﬁc energy, which is less competitive than today’s Li-electrodes (~600 Wh kg−1 for LiCoO2-type materials), hence the various attempts to boost the capacity of NVPF electrodes. Aﬁrst approach has consisted in the successful and reversible electrochemical insertion of 0.5 sodium ion in Na3V2(PO4)2F3 or 1 sodium ion in Na3V2(PO4)2O2F at potentials of ~1.6 V, respectively15–17. Such a low potential limits
the speciﬁc energy gain associated to the insertion of extra sodium ions but in contrast provides the feasibility to use Na3+x V2(PO4)2F3 composites as a sodium reservoir, as previously demonstrated, to compensate for the sodium loss at the carbon negative electrode during theﬁrst cycling15.
Another obvious path to increase the speciﬁc energy of NVPF
consists in harnessing the remaining sodium
(Na1V2(PO4)2F3–Na0V2(PO4)2F3) at high potential so as to reach theoretical energy densities of ~800 Wh kg−1. A signiﬁcant amount of research effort has been directed toward this goal, but have remained unproductive in accordance with density func-tional theory calculations stating that the removal of the third sodium ion should occur at potential (>4.9 V) that is too high for present electrolytes18,19. The accessibility of the third sodium ion in NVPF was thus remaining an open question.
Inadvertently, in our search toward exploring better electro-lytes for the NVPF/C sodium ion system20 we observed, by prolonged charging time at high potential, the feasibility to modify the voltage-composition proﬁle of the charge/discharge curve (e.g smoothing of the voltage features), hence providing a hint of some sodium electrochemical activity at high potential (Supplementary Figure 1). This inspired us to undertake a deeper exploration of Na3V2(PO4)2F3oxidation at high voltage.
Here in this work, we demonstrate the feasibility to electro-chemically remove nearly three sodium ions upon oxidation till 4.8 V vs Na+/Na0 with the concomitant formation of a new disordered “NVPF” phase that can reversibly uptake and release around three sodium ions on the following cycle; two between 4.2 and 3.6 V and the last one at 1.6 V. This provides a 20% gain in speciﬁc energy for NVPF/C sodium ion cells. We also
demonstrate the beneﬁts of the low voltage plateau to secure the use and the storage of such cells down to zero volts, and the feasibility of monitoring the state of charge (SoC) thanks to the S-shape proﬁle of the voltage-composition curves. Our ﬁndings offer unprecedented insight into the development of highly per-forming sodium ion systems.
Activating the third sodium in Na3V2(PO4)2F3 electro-chemically. Pristine single-phase Na3V2(PO4)2F3 material, as deﬁned by complementary X-ray diffraction (XRD), scanning electron microscopy, and inductive plasma analysis (ICP), was prepared via a two-step procedure as described in ref.21. Figure1
compares the voltage-composition curves and cycling perfor-mances of various NVPF/Na cells charged by limiting the amount of extracted sodium ions (Δx) to 2.0, 2.25, 2.5, 2.75, and 3.0 to produce samples that from now on will be referred to as NVPF-2, NVPF-2.25, NVPF-2.5, NVPF-2.75, and NVPF-3.0 respectively, and then discharged to 3.0 V. The proﬁle difference between the ﬁrst charge and subsequent discharge curve increases with Δx and becomes the most pronounced for Δx = 3.0. This suggests an electrochemical-driven irreversible structural change during the ﬁrst charging process, but once the ﬁrst cycle is achieved, sub-sequent charges and discharges superimpose. Note also a smoothing of the stair-case discharge curve forΔx = 2.0 (Fig.1a left) with increasing Δx that can be equally visualized on the corresponding derivative dQ/dV plots (Fig.1a right). Such a shift from a stair-case to an S-type voltage proﬁle is usually viewed as a positive asset for better SoC monitoring of the cell via the battery management system while obviously the decrease in potential is viewed as a negative asset for high-energy density. Whatever the amount of extracted sodium, only two sodium ions can be reversibly inserted, or slightly less for theΔx = 3.0 sample that also shows the more pronounced capacity decay (Fig.1b). Note that in neither case the kinetics of the reversible process seems to be affected as the power rate traces neatly superimpose irrespective ofΔx (see Supplementary Figure 2). The sodium content for the variousΔx samples at the end of charge was determined both by Electron Diffraction X-ray analysis (EDX) (Supplementary Figure 3) and ICP on electrodes recovered from the cells, which were washed and dried. These values converge with those deduced from coulometric titration at ±7%, overall three sodium ions are extracted on charge while solely two can be reinserted down to 3.0 V, hence the question of the missing one sodium ion.
To address this point, another set of ﬁve NVPF/Na cells were charged identically as the ﬁrst ones but discharged to 1.0 V. Importantly, the amplitude of the low voltage plateau (1.6–1.3 V) previously spotted for NVPF (here NVPF-2) is now enlarged with increasing Δx (Fig. 2a). Strikingly, its increasing amplitude nicely matches with the extra amount of sodium ions extracted beyond Δx = 2.0 as shown in the inset of Fig. 2a, as if there was a transfer from the high (~4.75 V) to the low voltage plateau (~1.6 V). When cycled between 4.4 and 1.0 V, the NVPF-3.0 sample shows a reversible electrode capacity of 200 mAh g–1 (Fig. 2b) as compared to 107 mAh g−1 when the cycling is limited between 4.4 and 3.0 V, in addition a more sustained capacity retention for the larger (4.4–1.0 V) cycling voltage range (Fig.2c vs. Fig. 1b). This ~40 % gain in capacity translates into solely ~15% beneﬁt in energy density because most of the extra discharge capacity is delivered at a low potential (Supplementary Figure 4). Still, this new polymorph exhibits the highest energy density reported so far among the NVPF compounds or their oxygenated variants (see Supplementary Table 1).
At this stage, a delicate question is to understand the origin of the large voltage drop when inserting the third sodium ion on
discharge. Obviously it is not related to the vanadium redox couple as it occurs upon reduction of both Na3V2(PO4)2F3and Na3V2(PO4)2FO2 independently of the involved couples are V3+/V2+ and V4+/V3+15,16. In contrast, previous studies have proposed that it could be due to changes in sodium mobility/ diffusivity19,22. To check this point, galvanostatic intermittent
titration-technique (GITT)-type measurements, which combine current pulses and open-circuit sequences, were performed during the second cycle for the NVPF-2.75 (Fig. 3). From the potential jump observed immediately after the application of the current pulse by ~1 s, we could deduce the variation of the cell resistance, which encompasses short-time-constant phenomena, such as electrolyte, electronic contact resistance, and charge transfer resistances. It shows an increase during discharge that is not correlated with the sudden potential drop. Moreover, changing the carbon concentration (10 or 50%) had no effect on the potential drop, therefore deﬁnitely ruling out possible electronic limitations across the conductive matrix of the electrode, as shown in Supplementary Figure 5. In contrast, there is just after the potential drop (Fig. 3), a markedly increase of the potential relaxation during the open circuit voltage (OCV) steps, which indicates a long-time-constant phenomena corresponding to the
slowed down diffusion of sodium ion in the solid phase. Since kinetics does not explain the voltage drop, it likely originates from thermodynamics. The plot of the potential after relaxation as a function of sodium stoichiometry (shown as a dashed line in Fig. 3) shows a hysteresis with different traces on charge and discharge, which point toward different reaction pathways. Thus, the question arises on how the NaxV2(PO4)2F3 structure accommodates the uptake and removal of sodium ions.
Structural evolutions when activating the third sodium in Na3V2(PO4)2F3. To address this point, ex situ synchrotron XRD measurements were performed on samples recovered from cells that were charged toΔx = 2.0, 2.25, 2.5, 2.75, and 3.0 and on two other sets of cells that were similarly charged and subsequently discharged to 3 and 1 V, respectively. The powder was placed in 0.7 mm glass capillaries and XRD patterns, as shown in Fig. 4, were recorded in transmission mode at the 11BM synchrotron beamline at Argonne National Laboratory with a wavelength of 0.412 Å. The pristine Na3V2(PO4)2F3 sample can be reﬁned successfully with the Rietveld method (Supplementary Figure 6) in the orthorhombic Amam space group with lattice parameters 0 25 120 80 40 120 80 40 120 80
Discharge capacity (mAh g
–1 ) 40 120 80 40 120 80 40 0 –25 25 0 –25 25 0 –25 25 0 –25 25 0 –25 –48 Δx = 3.0 Δx = 2.75 Δx = 2.75 3.70 Hardly be defined Hardly be defined 3.73 4.19 4.20 4.71 3.70 3.73 4.17 4.21 4.72 3.70 3.72 4.18 4.20 4.71 4.16 3.64 3.61 NVPF-3.0 NVPF-2.75 NVPF-2.5 Δx = 2.25 3.71 3.73 4.18 4.20 4.71 4.17 3.65 4.08 3.63 NVPF-2.25 Δx = 2.0 3.70 3.73 4.18 4.20 4.17 3.65 4.11 3.63 NVPF-2.0 4.8 a b 4.0 3.2 4.8 4.0 3.2 4.8 4.0 V oltage (V vs Na +/Na 0) dQ/dV (mAh g –1 V –1 ) 3.2 4.8 4.0 3.2 4.8 4.0 3.2 0 5 10 15 20 25 1 2 3 0 0 5 10 Cycle number 15 20 25 NVPF-2.0 NVPF-2.25 94% 124 mAh g–1 NVPF-2.5 86% 116 mAh g–1 NVPF-2.75 88% 104 mAh g–1 NVPF-3.0 74% 107 mAh g–1 97% 120 mAh g–1 1
X in NaxV2(PO4)2F3 Voltage (V vs Na+/Na0)
3.4 3.6 3.8 4.2 4.5 4.8
3.4 3.6 3.8 4.2 4.5 4.8
Fig. 1 Electrochemical characterization of NVPF samples in NVPF/Na half cells at a current of C/10 and cycled between 4.4 and 3.0 V. Theﬁrst charge process alone is controlled by limiting the amount of Na+extracted (Δx = 2.0, 2.25, 2.50, 2.75, and 3.0). a Voltage-composition curves (left) and their corresponding dQ/dV curves (right). b The corresponding capacity retention plots
a= 9.02976(14) Å, b = 9.04367(14) Å, and c = 10.75371(9) Å, in agreement with previous reports21,23. Partial views of the reﬁned
structure are shown in Fig.5. NVPF exhibits a three-dimensional structure built on V2O8F3 bi-octahedra bridged by PO4 tetra-hedra, and sodium occupies three interstitial sites: Na1 (pyr-amidal) fully occupied, and Na2 (pyr(pyr-amidal) and Na3 (capped prism) being partially occupied. In this structure, V is distributed on two crystallographic sites, which are similar in terms of environment and distances, and consistent with V3+ (average distance 1.98 Å, Fig.5).
The charged samples show a pronounced evolution of XRD patterns with increasing Δx that can easily be spotted at low θ angles (Fig. 4a left). All Rietveld reﬁnements are shown in
Supplementary Figure 7 with the corresponding Supplementary Tables 2 to 7 gathering all deduced structural parameters. First, let us note that the observed phase upon sodium extraction untilΔx = 2 perfectly agrees with early literature report23. Na1V2(PO4)2F3
presents a pattern that can be indexed in a Cmc21space group with lattice parameters a= 8.81577(19) Å, b = 8.8288(3) Å, and c = 11.00215(16) Å (V= 856.32 Å3 and V/Z= 214.08 Å3). In this structure, vanadium atoms are distributed on two crystallographic sites, each corresponding to V3+and V5+ oxidation states, while sodium occupies a single pyramidal site with full occupancy (Fig.5). The further oxidized sample (Δx = 2.25) shows a similar pattern that also can be indexed in Cmc21with however slight changes in lattice parameters (a= 8.8416(4) Å, b = 8.8567(5) Å, and c = 10.9804(3) Å), which reﬂects a decrease of sodium occupancy. For Δx = 2.5 and above, there is appearance of new peaks that progressively grow when Δx is increased, reﬂecting the presence of a mixture of the Cmc21phase and a new one. ForΔx = 3, this new phase appears as a single phase with an approximate chemical composition Na0V2(PO4)2F3 and its XRD pattern can be indexed with a tetragonal cell in space group I4/mmm, and lattice parameters a= 6.19887(18) Å and c = 11.3865(8) Å. The unit cell 4.8 a c b 4.5 3.0 1.5 4.5 3.0 1.5 4.5 3.0 1.5 4.5 3.0 1.5 4.5 3.0 1.5 NVPF-3.0 1.3 1 0.9 0.75 0.5 0.6 0.250.3 0 0.0 0 5 10 15 0 1 2 3 Cycle number 20 25 0.5 1.0 1.5 X in NaxV2(PO4)2F3 X in NaxV2(PO4)2F3 2.0 2.5 3.0 NVPF-2.0NVPF-2.25NVPF-2.5NVPF-2.75NVPF-3.0 0.1 NVPF-2.75 NVPF-2.5 Δx of Na at ~4.75 V NVPF-2.0 Δx of Na at ~1.6 V Δx of Na at ~4.75 V Δx of Na at ~1.6 V NVPF-2.25 3.6 V oltage (V vs Na +/Na 0) V oltage (V vs Na +/Na 0) 2.4 1.2 200 NVPF-2.0 NVPF-2.25 NVPF-2.5 NVPF-2.75 NVPF-3.0 150 100
Discharge capacity (mAh g
–1) 50 NVPF-2.0 140 mAh g–1 Δx = 2.21 NVPF-2.25 151 mAh g–1 Δx = 2.41 NVPF-2.5 167 mAh g–1 Δx = 2.67 NVPF-2.75 180 mAh g–1 Δx = 2.82 NVPF-3.0 200 mAh g–1 Δx = 3.13
Fig. 2 Electrochemical characterization of NVPF samples in NVPF/Na half cells cycled between 4.4 and 1.0 V. a First cycle activation in which the charging potential is used up to 4.8 V and charge process controlled by limiting theΔx (Na) = 2.0, 2.25, 2.50, 2.75, and 3.0 extracted, followed by discharge to 1 V at C/10. The inset shows the amount of Na+extracted at ~4.75 V and reinserted at ~1.6 V.b The charge-discharge proﬁle of the subsequent second cycle in the voltage window of 4.4 and 1.0 V.c The corresponding capacity retention plots
volume is 437.53(3) Å3and corresponds to V/Z= 218.76 Å3. This increase, compared to the sample forΔx = 2, arises from a larger c lattice parameter reminiscent of stronger electrostatic repulsions that are no longer screened by sodium atoms. The Rietveld reﬁnement for Δx = 3 is shown in Supplementary Figure 7 with the resulting structural parameters listed in Supplementary Table 3. This structural description enlists only one crystallographic site for V, and reﬁned V–O and V–F bond lengths (average bond length 1.87 Å) indicate an oxidation state of V in agreement with the expected value of 4.5+, as also conﬁrmed by bond valence sum calculations. Through discharge down to 1 V, the Δx = 2.0, 2.25, and 2.5 phases convert back to the Amam structure of the pristine material further conﬁrming the reversibility of the system within the 4.4–1.0 V voltage range (Fig.4b). Interestingly, the Δx = 2.75 and 3 samples stand as exceptions, since they never convert back into the pristine Amam phase as shown in Fig. 4b and Supplementary Figure 8. On the opposite, their patterns can be indexed in the tetragonal I4/mmm space group, as for the charged phases, and having sodium in a disordered state (i.e. Na occupies several Wyckoff sites with partial occupancy). These disordered reduced phases present the same symmetry and crystal structures (Na distribution) as the high temperature form of Na3V2(PO4)2F321. In this structure, Na atoms occupy two crystallographic sites (Wyckoff sites 8h and 16l) that form a circle aroundﬂuorine atoms (Fig.5). Reﬁning occupancies lead to 2.4 Na per formula unit when
the discharge is limited to 3 V, and 3.25 Na when the discharge is pursued down to 1 V (see Supplementary Tables 4 and 5). Consistently, the unit cell volume of the disordered phase V/Z= 222.87 Å3 is larger than that of the pristine one V/Z= 219.54 Å3 and of NVPF-2.0 discharged back to 1 V (V/Z= 220.57 Å3), respectively.
Evidence of sodium disorder in the newly formed tetragonal phase. To further characterize the extent of disorder in the structure and its origin, we recorded the 23Na and 31P magic
angle spinning-nuclear magnetic resonance spectra of ﬁve sam-ples: pristine NVPF, NVPF-2.5, NVPF-3.0 discharged to 3.0 and 1.0 V, and NVPF-2.0 discharged to 1.0 V (Fig.6). The shifts of the NMR resonance in these samples are Fermi contact shifts, which results from the presence of unpaired electrons on V3+or V4+ ions. Therefore, 31P NMR probes the state of the four neigh-boring vanadium ions, while23Na NMR provides a signature of the oxidation states of the two adjacent vanadium ions although sodium mobility and electron hoping may affect the observed spectra. Upon charging, the “narrow” 23Na and31P lines (sur-rounded by V3+ions in pristine NVPF, Fig.6a, f) have reduced shifts upon removal of vanadium electrons (Fig. 6e, j)24,25. A
detailed analysis is provided in the Supplementary Note 1. The main conclusion that can be drawn from the NMR analysis results from the comparison of the spectra of pristine NVPF and NVPF-2.0 discharged to 1 V (i.e. Fig.6a, f, e, j), and of NVPF-3.0 discharged to 3 and 1 V (Fig. 6c, d, h, i). On the one hand, it clearly conﬁrms, as observed before, that NVPF-2.0 returns to its original ordered state upon discharge. On the other hand, for NVPF-3.0 upon discharge, the broad distributions of environ-ments in 23Na and 31P spectra results from a distribution of vanadium oxidation states associated with sodium site occu-pancies, which are responsible for the variety of Fermi contact shifts on the neighboring phosphate groups and sodium ions, thereby conﬁrming the nature of the observed disorder. Alto-gether, NMR results unambiguously conﬁrm the presence of sodium disorder in the Na3V2(PO4)2F3 phase formed by initial removal of three sodium ions.
Charge compensation mechanism upon three sodium ions extraction/insertion. To recap the overall picture of the structural changes involved here, a tetragonal phase of approximate compo-sition Na0V2(PO4)2F3is formed when more than 2.5 sodium ions are extracted. Upon discharge, this phase accommodates sodium in a disordered way and does not convert back to the initial structure, further conﬁrming that upon oxidation we prepared a new type of NVPF. This phase can uptake reversibly nearly three sodium ions with limited volume change (ΔV/V = 3.0%) as deduced by in situ XRD (Supplementary Figure 9) hence accounting for the good cyclability of the material. Thus, a question that arises concerns now is the origin of this disorder. Equally important is the charge compensation mechanism occurring through this reversible pro-cess, which is the evolution of the V oxidation state that we could not access directly by XRD as it only gives hints through V–O and V–F distances.
To get further insights into the evolution of the V oxidation state upon Na extraction-insertion, X-ray absorption spectra (XAS) was measured at the V L-edge and O K-edge for ex situ samples at Na contents referred by an asterisk on the voltage-composition curve (Fig. 7a). The normalized spectra acquired in total ﬂuorescence yield (TFY) mode are presented in Fig.7b, c. The V L-edges for the pristine NVPF show two peaks at 517.5 and 523.5 eV, which can be ascribed to the L2/L3 splitting with the additional multiplet effect originated from large 2p-3d and 3d-3d Coulomb and exchange interactions, as suggested by Abbate et al. for V2O3and V2O526. During charge, the existing
peaks progressively shift to higher energies from 524.0 to 524.5 eV for instance, indicative of the vanadium oxidation since we observed a similar evolution when comparing with reference spectra taken on V2O3, Na1V2(PO4)3and V2O5 having V at the 3+, 4+, and 5+ oxidation states, respectively (Supplementary Figure 10). These signals shift back during discharge, showing the reduction of vanadium back to the original valence, hence further conﬁrming a reversible process. To gain further insight into the changes in electronic structure, we turn to the O K-edge reported 4 3 2 2 3 C/10 C/500 C/100 4 1 3 2 1 0 60 90 Ohmic resistance (m Ω ) 120 150 0.0 0.6 1.2 1.8 2.4 3.0 X in NaxV2(PO4)2F3 X in NaxV2(PO4)2F3 V o ltage (V vs Na +/Na 0) V oltage (V vs Na +/Na 0)
Fig. 3 Galvanostatic intermittent titration-technique (GITT) test of NVPF-2.75 sample after theﬁrst formation cycle. The cell was cycled at C/10 rate and the relaxation time was controlled either by 4 h or by limiting dV/dt < 0.1 mV/s; The red and blue solid lines show the experimental GITT curve on charge and discharge respectively, with the black dashed line showing the equilibrium potential after each relaxation process. The red and blue ﬁlled circles represent the Ohmic resistance at each point on charge and discharge process respectively. The inset shows NVPF-2.75/Na cell cycled at C/10, C/100, and C/500 within the range of voltage drop during theﬁrst discharge process
in Fig. 7c, where the most relevant feature lies in the pre-edge signal. It is associated to the transition from O(1s) to the antibonding V(3d)–O (2p) hybridized levels and the intensity is related to the V–O covalence26. Since V–O covalence increases
with the oxidation state of vanadium, the intensity of the pre-edge indirectly gives information on the valence of the vanadium atoms. The pre-edge signal shows a clear intensity increase/ decrease upon sodium ion removal/uptake, indirectly conﬁrming the oxidation/reduction of vanadium, through the whole process between 4.8 and 1 V.
While we demonstrated a change in V valence, we noted the appearance of a well-deﬁned peak at the O K-edge consistent with the emergence of a single valence and environment of V on
charging. This observation is consistent with a recent synchrotron XRD studies21reporting the disproportionation of V4+into equal
amounts of V3+and V5+in Na1V2(PO4)2F3. Byﬁtting the pre-edge signals of the O K-pre-edge collected for our Na1V2(PO4)2F3 with four Gaussian peaks at 529.3, 531.5, 531.9, and 533.3 eV, we form two sets of doublets corresponding to V5+(529.3–531.9 eV) and V3+ (531.5–533.3 eV). This treatment was extended to all samples and we plotted the variation of the V5+/V3+signal ratio upon Na extraction (see Supplementary Figure 11 and Supple-mentary Tables 8, 9). It continuously increases upon extraction suggesting that the V4+disproportionation happens all along the extraction process with the opposite variation occurring during discharge, except from a small shift of the V5+t2gstate. This shift
Intensity (a.u.) Intensity (a.u.) NVPF-3.0 a b I4/mmm NVPF-3.0 discharge 1V I4/mmm NVPF-2.75 I4/mmm NVPF-2.75 discharge 1V I4/mmm NVPF-2.5 Cmc21 + I4/mmm NVPF-2.5 discharge 1V Amam NVPF-2.25 discharge 1V Amam NVPF-2.0 discharge 1V Amam NVPF-2.25 Cmc21 NVPF-2.0 3.5 4.0 2 ( = 0.412 Å) 2 ( = 0.412 Å) 2 ( = 0.412 Å) 4.5 5 6 7 8 9 10 12 14 16 18 20 3.5 4.0 2 ( = 0.412 Å) 2 ( = 0.412 Å) 2 ( = 0.412 Å) 4.5 5 6 7 8 9 10 12 14 16 18 20 Cmc21
Fig. 4 Structural evolutions during three sodium ions extraction/insertion in NVPF. a Synchrotron X-ray diffraction patterns of the charged samples with different amounts of Na extracted (NVPF-2.0, NVPF-2.25, NVPF-2.5, NVPF-2.75, and NVPF-3.0).b The other set of samples further discharged down to 1 V
can be attributed to an increase in the number of sodium NVPF pristine * * * * NVPF-2.5 NVPF-3.0 discharge 3.0 V NVPF-3.0 discharge 1.0 V NVPF-2.0 discharge 1.0 V 400 e d c b a j i h g f 300 200 100 0 23Na (ppm) 31P (ppm) –100 –200 –300 –400 8000 6000 4000 2000 0
Fig. 6 NMR spectroscopic evidence of sodium disorder in NVPF. a–e23Na andf–j31P magic angle spinning-nuclear magnetic resonance spectra after a Hahn echo sequence recorded at 4.7 T and a spinning rate of 50 kHz.a, f Pristine NVPF. b, g NVPF-2.5. c, h NVPF-3.0 discharged to 3.0 V. d, i NVPF-3.0 discharged to 3.0 V and 1.0 V respectively.e, j NVPF-2.0 discharged to 1.0 V. The stars indicate spinning sidebands, the red arrow shows a small contribution from neighboring V4+ions in the pristine NVPF. The dashed lines are guide for the eyes. The23Na spectra are shown without modiﬁcation, while the31P spectra levels were adjusted for clarity
NVPF Na3V2(PO4)2F3 1.97 Å F2 F1 F2 Na1 Na1 Na2 Na2 Na2 Na2
Na1Na2Na2Na1 Na2 Na2 Na2 Na2 Na1 Na1 Na2 Na2
Na1Na2Na2Na1 Na2 Na2 Na2 Na2 Na1 Na1 Na2 Na2 Na2 Na1 Na2 Na3 Na3 Na3 Na3 Na1 F3 F1 F2 F2 F2 F2 F1 F1 F1 F2 F2 F2 V1 V2 1.97 Å <d > = 1.98 Å
Amam Cmc21 I4/ mmm I4/ mmm I4/ mmm
<d1> = 1.95 Å <d > = 1.87 Å <d > = 1.97 Å <d > = 2.00 Å <d2> = 1.86 Å 1.98 Å 1.98 Å 2.04 Å 1.61 Å 1.87 Å 2.01 Å 1.62 Å 1.62 Å 1.92 Å 1.92 Å 1.92 Å 1.92 Å 1.98 Å 1.98 Å 1.94 Å 1.94 Å 1.99 Å 1.99 Å NVPF-2.0 Na1V2(PO4)2F3 NVPF-3.0 Na0V2(PO4)2F3 NVPF-2.75 discharged to 3V NVPF-2.75 discharged to 1V
Fig. 5 V–F bond lengths and sodium distribution within the structure of NVPF samples. Structures of NVPF samples, from left to right: pristine, NVPF-2.0, NVPF-3.0, NVPF-2.75 discharged to 3.0 V, and NVPF-2.75 discharged to 1.0 V. Top: view of the VO8F3bioctahedra with relevant V–F bond lengths and the
average V–O/F distances labeled as <d>; bottom: distribution of Na atoms within the structure. For each composition, the space group is indicated. V is blue, O is red, F is gray, Na is yellow, and Na vacancies are milky white
neighbors, which will change the Madelung energy and shift the V5+peak, in agreement with XRD data.
Electrochemical performance of NVPF/C full cells by utilizing the third sodium in NVPF. Next, we have implemented the aforementioned fundamental/experimental knowledge to the assembly of optimized NVPF/C cells. Figure8 illustrates the per-formances of full cells, having a mass ratio positive to negative electrode of 2, and using an increasing fraction of the third plateau capacity during theﬁrst cycle. The cells cycled between 4.3 and 2 V show an increase in capacity from 107 to 121 mAh g–1 for the NVPF-2.5 as compared to NVPF-2.0 as shown in Fig.8a. The extra capacity gained by utilizing about half of this new third plateau translates into a ~14% increase in energy (396–451 Wh kg−1based
on the mass of NVPF), while preserving excellent capacity retention (Fig.8b). Within this context, it is worth recalling that the highest achievable energy will depend on the value of the mass ratio of positive to negative (r), the voltage scanning domain, and the amount of sodium removed on the third plateau during the ﬁrst charge. For instance, the maximum beneﬁts in terms of capacity and energy when cycling over the 4.3–2 V voltage range is obtained with NVPF-2.6 sample using a NVPF/C mass ratio of 1.98 (Sup-plementary Figure 12), which is for instance 2% higher than what can be achieved with NVPF-2.5 using a mass ratio of 2.06 (Sup-plementary Figure 12). Note also that we can recover the signature of the low voltage plateau pertaining to the NVPF positive electrode by lowering the full cell voltage to zero volt. In that case, with r= 2, the increase in energy density approaches ~18% for NVPF-2.75 with respect to NVPF-2, but it must be recognized that some of the 5.0 a b c 4.5 4.0 3.5 3.0 1.2 0.9 0.6 0.3 0.0 5 4 3 2 1 3.0 513 530 532 534 536 538 540 542 528 531 534 537 540 543 516 519 Energy (eV)
Energy (eV) Energy (eV)
Energy (eV) 522 525 513 516 519 522 525 2.5 2.0 1.5 1.0 0.5 0.0 0.5 1.0 1.5 2.0 2.5 3.0 3.5 X in NaxV2(PO4)2F3 V o ltage (V vs Na +/Na 0) Nor maliz ed intensity (a.u.) 1.2 0.9 0.6 0.3 0.0 Nor maliz ed intensity (a.u.) 1.2 0.9 0.6 0.3 0.0 Nor maliz ed intensity (a.u.) 1.2 0.9 0.6 0.3 0.0 Nor maliz ed intensity (a.u.) V o ltage (V vs Na +/Na 0) X in NaxV2(PO4)2F3 Na1.5VPF Na1.5VPF Na1.5VPF Na0.75VPF Na0.75VPF Na0.75VPF Na2.0VPF Na2VPF Na2VPF Na3.3VPF Na3.3VPF Na3.3VPF 516.7 518.5 524.5 Na0.25VPF Na0.25VPF Na0.25VPF NVPF-3.0 516.7 529.3 - V5+ 529.3 - V5+ 531.9 - V5+ 531.9 - V5+ 533.3 - V3+ 531.5 - V3+ 533.3 - V3+ 531.5 - V3+ 518.5 524.5 NVPF-2.0 NVPF-2.0 NVPF-1.0 NVPF-1.0 NVPF-3.0 NVPF-3.0 NVPF-2.0 Pristine Pristine Pristine Charge
Charge-V L edge Discharge-V L edge
Charge-O K edge Discharge-O K edge
Fig. 7 Evolution of the vanadium oxidation state upon Na+extraction/insertion.a The voltage-composition curve of NVPF-3.0 sample cycled at C/10 in which the experimental points used for ex situ X-ray absorption analysis are marked with the respective Na-stoichiometry. The normalized (b) V L-edge andc O K-edge X-ray absorption spectra of the corresponding charge (left) and discharge (right) samples obtained in totalﬂuorescence yield mode
extra-gain comes from the low-voltage plateau, which application-wise is not the most attractive. Altogether, these results unam-biguously prove the energy density beneﬁts of partially or wholly harvesting the third sodium ion from NVPF.
Lastly and worth stressing is the low-voltage plateau occurring at 1.6 V in NVPF/Na cell, which is shifted to 0.9 V in NVPF/C full cells, with its amplitude increasing as Δx increases. To fully explore this low-voltage domain, two cells were previously charged toΔx = 2 and 2.75, and then cycled ﬁve times between 4.3 and 2.0 Vﬁrst, and maintained at zero volts for 1 week prior
to be recharged and cycled again over the 4.3–2 V voltage domain. Note that the NVPF-2 loses 4% of its capacity during the 0 V resting period, while no capacity lost is observed for NVPF-2.75 sample (Fig.8d and Supplementary Figure 13). Most likely, the low-voltage plateau serves as a buffer to clamp the voltage of both the NVPF positive and carbon negative electrodes to lower values so as to minimize side reactions during the over-discharge tests. From a practical perspective, this low-voltage plateau is an inherent asset for facilitating the handling (transport and storage of cells at zero volts) of NVPF/C sodium ion cells without 4.5 a b c d 120 4.5 3.6 2.7 1.8 V oltage (V) 0.9 0.0 100 Capacity (mAh g –1 ) 80 105 90 75 60
Discharge capacity (mAh g
–1 ) Energy density (Wh kg –1 ) 45 30 15 0 150 300 450 Energy density (Wh kg –1 ) 0 150 300 450 396 441 94% 451 95% +14% 443 91% 95% 418 389 427 450 458 +18% 444 77% 0 0 0.0 0.5 1.0 1.5 2.0 2.5 3.0 20 40 Cycle number
Cycle number (arb. units) Before 0 V
Over-discharge Over-dischargeAfter 0 V
60 80 100 3.6 2.7 1.8 0.9 0.0 4.5 3.6 2.7 1.8 0.9 0.0 4.5 3.6 2.7 1.8 0.9 0.0 4.5 3.6 2.7 1.8 0.9 0.0 4.5 3.6 2.7 1.8 0.9 0.0 0.0 0.5 1.0 1.5 2.0 2.5 3.0 V oltage (V vs Na +/Na 0) X in NaxV2(PO4)2F3 X in NaxV2(PO4)2F3 NVPF-2.0 NVPF-2.0 107 mAh g–1 Δx = 2.0 NVPF-2.25 NVPF-2.25 NVPF-2.0 120 mAh g–1 Δx = 2.25 NVPF-2.75 NVPF-2.75 119 mAh g–1 Δx = 2.75 NVPF-3.0 NVPF-3.0 NVPF-2.75 Buffer 111 mAh g–1 Δx = 3.0 NVPF-2.5 NVPF-2.5 121 mAh g–1 Δx = 2.5 NVPF-2.0NVPF-2.25NVPF-2.5NVPF-2.75NVPF-3.0 NVPF-2.0NVPF-2.25NVPF-2.5NVPF-2.75NVPF-3.0 NVPF-2.0 NVPF-2.25 NVPF-2.75 NVPF-3.0 NVPF-2.5
Fig. 8 Electrochemical performance of NVPF/C full cells. The voltage-composition curves a and cycling performance b of NVPF/C full cell of NVPF-2.0, 2.25, 2.5, 2.75, and 3.0 samples cycled between 4.3 and 2.0 V afterﬁrst activation process up to 4.8 V at C/10 followed a potentiostatic charging until reaching the exact amount of Na+content, where insets inb is the histogram of the discharge energy density based on the mass of NVPF. c The voltage-composition curves of NVPF/C full cell of NVPF-2.0, 2.25, 2.5, 2.75, and 3.0 sample cycled down to 0 V with the inset showing the histogram of energy density based on the mass of NVPF.d The cycling performance of NVPF-2.0 and NVPF-2.75 in a full cell before and after zero volt over-discharge tests for 1 week
prejudice in their following uses, which is not the case with the Li-ion technology for instance.
The results reported here introduce the feasibility to reversibly remove, in contrast to previous beliefs, the third sodium ion from NVPF, hence offering this material and the resulting NVPF/C ion cells an additional asset for practical applications in terms of energy density and ability to be stored at 0 V without a performance penalty. Fundamental studies from complementary XRD, XAS, and electrochemical experiments establish that this extraction is asso-ciated with the oxidation of Vn+beyond 4+ and is concomitant with the formation, structurally wise, of a new tetragonal “NVPF” phase, which can reversibly uptake three sodium ions; two and one at high and low potentials, respectively. However, as it is often the case with new results in the area of energy storage, the fundamental science still needs to be understood. Speciﬁcally, what are the mechanisms for sodium ion extraction/uptake, sodium ion trans-port, and structural reacting paths? Some of these points are now discussed in light of our experimentalﬁndings.
Classical extraction/insertion processes usually lead to charge and discharge curves, which mirror each other. Such a condition is no longer satisﬁed here since the ﬁrst discharge proﬁle differs drastically from the charge one, once the third sodium is extracted from the NVPF structure. This leads to the irreversible formation of new “NVPF” disordered compound as deduced by XRD, which remains as such through subsequent cycling. Such a situation is not unique and has been observed in Li2FeSiO4and Li3VO4, where it was ascribed to the onset of a Li/M interstice mixing upon reduction27,28. Such a scenario is quite unlikely here owing to the large size difference between Na+and V5+. Another possibility would be a strengthening of the V= O bond at the expense of a lengthening of the V–F bond toward the end of the oxidation, making it more vulnerable toward bond breaking. This could lead to the formation of F vacancies having the possibility to permanently modify Na distribution. However, such a hypothesis could not be validated owing to our inability to (i) reach satisfactory Rietveld reﬁnements upon introduction of F vacancies and (ii) to detectﬂuorine by19F NMR in the electrolyte recovered from a cell that was fully charged using NaClO4rather than NaPF6-based electrolyte. Most likely, under strong oxidation conditions, we change the energy of the Na vacancy landscape via some subtle framework modiﬁcations, which cannot be clearly determined with powder XRD. This could promote permanently a more energetically favorable disordered Na path that, once formed, remains on subsequent cycles.
Turning to the evolution of the vanadium oxidation state upon Na+extraction/insertion, our XAS data together with bond valence sums deduced from XRD indicate that vanadium can reach an average oxidation state approaching 4.5+. However, ambiguity remains as whether oxidation states (V3+, V4+, and V5+) coexist within the same material. Their coexistence upon sodium extrac-tion was shown in Na3V2(PO4)2O1.6F1.4via X-ray absorption near edge structure spectroscopy29. In contrast, recent synchrotron
XRD studies, which we conﬁrmed by soft XAS, support the exis-tence of V disproportionation (2V4+→ V3++ V5+) in Na1V2 (PO4)2F3 that is associated with the instability of V4+in VO4F2 octahedrons23,25,30. These observations indicate the feasibility of
having V4+in O-substituted NVPF, but not in pure NVPF com-pounds having VO5−xFxand VO4F2octahedron. Let us recall that within the NVPF-type structure, V ions sit in the center of octa-hedra linked by vertices through ﬂuorine atoms to form V2O8F3 bioctahedra, while in the O-substituted phases, V2O8+xF3−x bioc-tahedra present V–O–V bonds along the c-axis. Obviously, the large predominance of V–F–V bonds in contrast to V–O–V bonds
will limit the possibility of stabilizing vanadyl groups. We thus believe that the difﬁculty in stabilizing V4+in theﬂuoride envir-onment provided by VO4F2 octahedron favors the dis-proportionation of V4+into V3+and V5+.
Having consolidated, based on complementary GITT and galvanostatic measurements, that the origin of the potential jump is not kinetic in nature, a question remains regarding the onset of this potential jump, which occurs at x= 2 in our newly dis-ordered NaxV2(PO4)2F3 phase instead of x= 3 in NVPF or O-substituted NVPF. A tentative answer can be deduced by considering the phase that forms at high potential during charge, which inﬂuences the discharge proﬁle with the amount of sodium release at high potential being nearly equal to that reinserted at low potential. Let’s note that the I4/mmm structure contains two different Na sites, A and B sites, that could be the Na2 and Na1 on Wyckoff positions 16l and 8h, respectively (Supplementary Tables 4 and 5). One can simply imagine that, ﬁrst, the A sites depopulate (Na3V2(PO4)2F3→ Na1V2(PO4)2F3) followed by the B sites at high potential, and then A sites reﬁll prior to the B sites so that the sodium ion liberated from B sites at ~4.7 V are solely reinserted at ~1.6 V. Such a scenario leads to different metastable intermediate states in agreement with the different thermo-dynamic reaction paths observed via GITT measurements. Moreover, it could then explain the need to have two reinserted sodium ions corresponding to A sites, whatever the amount of sodium ions extracted in charge, before the potential jump occurs. The large potential difference (~4.7− 1.6 = 3.1 V) between the depopulation/repopulation of B sites could be explained by dif-ferent sodium environments associated to difdif-ferent V(n+1)+/Vn+ redox couples. Further exploration of the sodium-driven local structural changes in NVPF by combined transmission electron microscopy, electron paramagnetic resonance, and operando XAS studies are needed to further support this scenario, since neither lab-XRD nor synchrotron sources can sort out differences between sites occupancies.
Overall, this study contradicts the conventional understanding of the electrochemical properties of Na3V2(PO4)2F3, by showing that the third sodium ion can be reversibly removed, which leads to a new polymorph having disordered rather than ordered sodium sites, and a tetragonal symmetry instead of an orthor-hombic one. We found that the amount of sodium ions removed mirrors the amount reinserted at low potential and explained this balance by the existence of two thermodynamic paths corre-sponding to different sites occupancies sequences. Furthermore, this report offers a new way to enhance the energy density of Na3V2(PO4)2F3batteries by 14% while preserving excellent cycle life and suitable rate capabilities for applications. Lastly, we demonstrate that the onset of the low insertion plateau con-stitutes a practical step toward the design of sodium ion cells having performances unaffected by maintaining or discharging the cell to zero volts. Hence, these novel insights should help in boosting the development of the sodium ion technology. Methods
Electrochemical characterization. Electrodes were mainly consisting either of 11 mm diameter disks punch out of Al supported calendared NVPF/Csp/PVDF tapes with a 92/4/4 in weight ratio and a loading of 12 mg cm–2. Powdered composite mixtures (NVPF/Csp with a 90/10 in weight ratio) were occasionally used. A unit of 1 M NaPF6(Stella, Japan) dissolved in PC (BASF, Germany) was used as the
elec-trolyte, glassﬁber (GF/D, Whatman) was used as separator, and sodium metal (Sigma-Aldrich) and hard carbon were used as negative electrode for half cells and full cells respectively, throughout the paper unless otherwise speciﬁed. In the initial stages of the exploration of the third plateau of NVPF (Supplementary Figure 1), the elec-trolyte 1 M NaPF6dissolved in PC/EC/DMC (1/1/1 in volume ratio) was used. The
Swagelok and coin-type cell were assembled in the glovebox (MBRAUN, Germany) either in half cells or full cells, in which the current density of C/10 (1C= 128 mA g–1) was applied by a MPG-2 or VMP-3 potentiostat (Bio-Logic, France). The potentio-static mode by limiting the current to less than C/100 at 4.8 V (vs. Na+/Na0) was only
employed in theﬁrst formation charge process. The GITT (every Δx = 0.1) was performed in the second cycle of NVPF-2.75 sample after theﬁrst activation cycle, and the relaxing process was controlled either by dV/dt≤ 0.1 mV s–1or 4 h.
Ex situ synchrotron XRD. First, the designed amount of sodium ions were extracted from or reinserted into the NVPF structure electrochemically in the Swagelok cell, and the recovered powder was washed with dimethyl carbonate (DMC) and dried in vacuum before sealing it in 0.7 mm glass capillaries for syn-chrotron XRD measurements. The ex situ synsyn-chrotron XRD measurements were performed using the mail in user facility at 11BM synchrotron beamline, Argonne National Laboratory (λ = 0.412 Ǻ). All Rietveld reﬁnements were performed using the FullProf program31.
Ex situ soft X-ray absorption. A series of charged and discharged samples (NVPF electrodes here) with certain amount of sodium ions extracted were prepared in the Swagelok type cell, and the cycled samples are washed, dried, and sealed in argon for XAS measurements before sealing in the bags made of Al-plasticﬁlm. Samples were then mounted in a glovebox and transferred under Argon environment into the beamline end station. The L-edge of V and O K-edge XAS spectra was obtained in both surface (total electron yield) and bulk sensitive (TFY) simultaneously at beamline 4-ID-C of the Advanced Photon Source. All spectra were aligned by the simultaneous measurement of an MgO reference sample.
Magic angle spinning-nuclear magnetic resonance. The spectra were recorded on a Bruker 4.7T (200 MHz for1H) double resonance spectrometer, operating at
53 MHz for23Na and 81 MHz for31P, using a 1.3 mm double resonance magic
angle spinning probe, with a spinning rate of 50 kHz, and N2for the bearing, drive,
and frame cooling gasﬂows. The 1.3 mm zirconia rotor were ﬁlled in a glovebox under Argon. The effective RFﬁeld strength was set to 250 kHz for23Na and31P,
using a Hahn echo sequence over two rotor periods (i.e. 40μs) to obtain a distortion-free baseline. In the case of31P, the spectra were recorded using variable
offset-cumulative spectrum—every 250 kHz—to record the complete signal32. The spectra wereﬁtted with DmFit for the quantiﬁcation of each peak when needed, using standard Gausso-Lorentzian peaks33. The spectra were referenced with a 1 M NaCl solution in water for23Na and 85% H3PO4in water for31P. The longitudinal
relaxation times T1’s were around 0.5 to a couple of milliseconds, and recycling
delays of 30 ms were used to ensure a complete recovery of the magnetization. For
23Na and31P, 4096 and 16,384 transients were recorded for each spectrum/offset,
and exponential line broadening of 500 and 2000 Hz were applied, respectively. Data availability
The data supporting theﬁndings of this study are available from the authors on reasonable request.
Received: 9 June 2018 Accepted: 21 December 2018
1. Dunn, B., Kamath, H. & Tarascon, J. M. Electrical energy storage for the grid: a battery of choices. Science 334, 928–935 (2011).
2. Yang, Z. G. et al. Electrochemical energy storage for green grid. Chem. Rev. 111, 3577–3613 (2011).
3. Larcher, D. & Tarascon, J.-M. Towards greener and more sustainable batteries for electrical energy storage. Nat. Chem. 7, 19–29 (2015).
4. Grey, C. & Tarascon, J. Sustainability and in situ monitoring in battery development. Nat. Mater. 16, 45–56 (2017).
5. Kubota, K. & Komaba, S. Review—practical issues and future perspective for Na-ion batteries. J. Electrochem. Soc. 162, A2538–A2550 (2015).
6. Pan, H. L., Hu, Y. S. & Chen, L. Q. Room-temperature stationary sodium-ion batteries for large-scale electric energy storage. Energy Environ. Sci. 6, 2338–2360 (2013).
7. Yabuuchi, N., Kubota, K., Dahbi, M. & Komaba, S. Research development on sodium-ion batteries. Chem. Rev. 114, 11636–11682 (2014).
8. Wang, P.-F., You, Y., Yin, Y.-X. & Guo, Y.-G. Layered oxide cathodes for sodium-ion batteries: phase transition, air stability, and performance. Adv. Energy Mater. 8, 1701912 (2017).
9. Ponrouch, A. et al. Towards high energy density sodium ion batteries through electrolyte optimization. Energy Environ. Sci. 6, 2361–2369 (2013). 10. Dugas, R., Zhang, B., Rozier, P. & Tarascon, J. M. Optimization of Na-ion
battery systems based on polyanionic or layered positive electrodes and carbon anodes. J. Electrochem. Soc. 163, A867–A874 (2016).
11. Park, Y. U. et al. A new high-energy cathode for a Na-ion battery with ultrahigh stability. J. Am. Chem. Soc. 135, 13870–13878 (2013).
12. Mu, L. et al. Prototype sodium-ion batteries using an air-stable and Co/Ni-Free O3-layered metal oxide cathode. Adv. Mater. 27, 6928–6933 (2015).
13. Gover, R., Bryan, A., Burns, P. & Barker, J. The electrochemical insertion properties of sodium vanadiumﬂuorophosphate, Na3V2(PO4)2F3. Solid State
Ion. 177, 1495–1500 (2006).
14. Chihara, K. et al. Cathode properties of Na3M2(PO4)2F3[M= Ti, Fe, V] for
sodium-ion batteries. J. Power Sources 227, 80–85 (2013).
15. Zhang, B. et al. Insertion compounds and composites made by ball milling for advanced sodium-ion batteries. Nat. Commun. 7, 10308 (2016).
16. Bianchini, M., Xiao, P., Wang, Y. & Ceder, G. Additional sodium insertion into polyanionic cathodes for higher-energy Na-ion batteries. Adv. Energy Mater. 7, 1700514 (2017).
17. Palomares, V. et al. Structural evolution of mixed valent (V3+ /V4 + ) and V4+ sodium vanadium ﬂuorophosphates as cathodes in sodium-ion batteries: comparisons, overcharging and mid-term cycling. J. Mater. Chem. A 3, 23017–23027 (2015).
18. Park, Y. U. et al. A family of high-performance cathode materials for Na-ion batteries, Na3(VO1-xPO4)2F1+2x(0≤ x ≤ 1): combined ﬁrst-principles and
experimental study. Adv. Funct. Mater. 24, 4603–4614 (2014).
19. Dacek, S. T., Richards, W. D., Kitchaev, D. A. & Ceder, G. Structure and dynamics ofﬂuorophosphate Na-ion battery cathodes. Chem. Mater. 28, 5450–5460 (2016).
20. Yan, G. et al. Assessment of the electrochemical stability of carbonate-based electrolytes in Na-ion batteries. J. Electrochem. Soc. 165, A1222–A1230 (2018). 21. Bianchini, M. et al. Na3V2(PO4)2F3revisited: a high-resolution diffraction
study. Chem. Mater. 26, 4238–4247 (2014).
22. Matts, I. L. et al. Explaining performance-limiting mechanisms in ﬂuorophosphate Na-ion battery cathodes through inactive transition-metal mixing andﬁrst-principles mobility calculations. Chem. Mater. 27, 6008–6015 (2015).
23. Bianchini, M. et al. Comprehensive investigation of the
Na3V2(PO4)2F3–NaV2(PO4)2F3system by operando high resolution
synchrotron X-ray diffraction. Chem. Mater. 27, 3009–3020 (2015). 24. Liu, Z. et al. Local structure and dynamics in the Na ion battery positive
electrode material Na3V2(PO4)2F3. Chem. Mater. 26, 2513–2521 (2014).
25. Broux, T. et al. Comprehensive investigation of the
Na3V2(PO4)2F3–NaV2(PO4)2F3system by operando high resolution
synchrotron X-ray diffraction. Chem. Mater. 28, 7683–7692 (2016). 26. Abbate, M. et al. Soft X-ray absorption spectroscopy of vanadium oxides.
J. Electron Spectros. Relat. Phenomena 62, 185–195 (1993).
27. Saracibar, A., Van der Ven, A. & Arroyo-de Dompablo, M. E. Crystal structure, energetics, and electrochemistry of Li2FeSiO4polymorphs fromﬁrst
principles calculations. Chem. Mater. 24, 495–503 (2012).
28. Li, H. et al. A promising insertion anode material for lithium-ion batteries. Adv. Energy Mater. 3, 428–432 (2013).
29. Serras, P. et al. Electrochemical Na extraction/insertion of Na3V2O2x(PO4)2F3–2x. Chem. Mater. 25, 4917–4925 (2013).
30. Broux, T. et al. VIV disproportionation upon sodium extraction from Na3V2(PO4)2F3observed by operando X-ray absorption spectroscopy and
solid-state NMR. J. Phys. Chem. C 121, 4103–4111 (2017).
31. Rodríguez-Carvajal, J. Recent advances in magnetic structure determination by neutron powder diffraction. Phys. B 192, 55–69 (1993).
32. Massiot, D. et al. 71Ga and 69Ga nuclear magnetic resonance study of β-Ga2O3: resolution of four- and six-fold coordinated Ga sites in static
conditions. Solid State Nucl. Magn. Reson. 4, 241–248 (1995). 33. Massiot, D. et al. Modelling one- and two-dimensional solid-state NMR
spectra. Magn. Reson. Chem. 40, 70–76 (2002).
J.-M.T. acknowledges funding from the European Research Council (ERC) (FP/2014)/ ERC, Grant-Project 670116-ARPEMA; Q.J. thanks the ANR“Deli-Redox” for Ph.D. funding. This research used resources of the Advanced Photon Source (11BM and 4-ID-C), a U.S. Department of Energy (DOE) Ofﬁce of Science User Facility operated for the DOE Ofﬁce of Science by Argonne National Laboratory under Contract No. DE-AC02-06CH11357. The authors thank M.-L. Doublet and C. Delacourt for fruitful discussion together with A. Abakumov and J. Hadermann for looking at some of the reported samples by TEM, and D. Giaume for ICP analysis. M.D. acknowledges support from CNRS and LabeX STORE-EX for funding.
G.Y., J.-M.T. and S.M. designed and conducted the experimental work. G.R. analyzed the crystal structure of all samples. M.D. performed the MAS-NMR experiments and ana-lyzed the data. R.D. synthesized the pristine material of Na3V2(PO4)2F3. Q.J. and J.F. participate in the acquisition and analysis of the soft X-ray absorption data. B.M. con-ducted the elemental analysis by EDX. All authors discussed the results and contributed to draft the manuscript.
Supplementary Informationaccompanies this paper at https://doi.org/10.1038/s41467-019-08359-y.
Competing interests:The authors declare no competing interests.
Reprints and permissioninformation is available online athttp://npg.nature.com/ reprintsandpermissions/
Journal peer review information: Nature Communications thanks the anonymous reviewers for their contribution to the peer review of this work. Peer reviewer reports are available.
Publisher’s note: Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional afﬁliations.
Open Access This article is licensed under a Creative Commons Attribution 4.0 International License, which permits use, sharing, adaptation, distribution and reproduction in any medium or format, as long as you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in a credit line to the material. If material is not included in the article’s Creative Commons license and your intended use is not permitted by statutory regulation or exceeds the permitted use, you will need to obtain permission directly from the copyright holder. To view a copy of this license, visithttp://creativecommons.org/ licenses/by/4.0/.